#------------------------------------------------------------------------------
#$Date: 2019-05-21 14:26:13 +0300 (Tue, 21 May 2019) $
#$Revision: 215354 $
#$URL: file:///home/coder/svn-repositories/cod/cif/2/10/35/2103518.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/. The original data for this entry
# were provided by IUCr Journals, http://journals.iucr.org/.
#
# The file may be used within the scientific community so long as
# proper attribution is given to the journal article from which the
# data were obtained.
#
data_2103518
loop_
_publ_author_name
'Pavlovska, A.'
'Werner, S.'
'Maximov, B.'
'Mill, B.'
_publ_section_title
;
 Pressure-induced phase transitions of piezoelectric single crystals
 from the langasite family: La₃Nb~0.5~Ga~5.5~O₁₄ and
 La₃Ta~0.5~Ga~5.5~O₁₄
;
_journal_issue                   6
_journal_name_full               'Acta Crystallographica Section B'
_journal_page_first              939
_journal_page_last               947
_journal_paper_doi               10.1107/S0108768102010273
_journal_volume                  58
_journal_year                    2002
_chemical_formula_sum            'Ga5.54 La3 O14 Ta0.46'
_chemical_formula_weight         1110.22
_space_group_IT_number           150
_symmetry_space_group_name_Hall  'P 3 2"'
_symmetry_space_group_name_H-M   'P 3 2 1'
_atom_sites_solution_hydrogens   geom
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-97
_cell_angle_alpha                90.00
_cell_angle_beta                 90.00
_cell_angle_gamma                120.00
_cell_formula_units_Z            1
_cell_length_a                   7.872
_cell_length_b                   7.872
_cell_length_c                   4.999
_cell_measurement_temperature    293(2)
_cell_volume                     268.3
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 1997)'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 1990)'
_diffrn_ambient_pressure         16.7E+6
_diffrn_ambient_temperature      293(2)
_diffrn_measured_fraction_theta_full 0.512
_diffrn_measured_fraction_theta_max 0.512
_diffrn_radiation_source         synchrotron
_diffrn_radiation_wavelength     0.56000
_diffrn_reflns_av_R_equivalents  0.0000
_diffrn_reflns_av_sigmaI/netI    0.0626
_diffrn_reflns_limit_h_max       15
_diffrn_reflns_limit_h_min       -15
_diffrn_reflns_limit_k_max       9
_diffrn_reflns_limit_k_min       -9
_diffrn_reflns_limit_l_max       8
_diffrn_reflns_limit_l_min       -8
_diffrn_reflns_number            841
_diffrn_reflns_theta_full        35.99
_diffrn_reflns_theta_max         35.99
_diffrn_reflns_theta_min         2.35
_exptl_absorpt_coefficient_mu    15.883
_exptl_crystal_density_diffrn    6.872
_exptl_crystal_density_method    'not measured'
_exptl_crystal_F_000             488
_refine_diff_density_max         4.591
_refine_diff_density_min         -4.098
_refine_diff_density_rms         0.584
_refine_ls_abs_structure_details 'Flack H D (1983), Acta Cryst. A39, 876-881'
_refine_ls_abs_structure_Flack   -0.26(17)
_refine_ls_extinction_coef       0.004(8)
_refine_ls_extinction_expression Fc^*^=kFc[1+0.001xFc²λ³/sin(2θ)]^-1/4^
_refine_ls_extinction_method     SHELXL
_refine_ls_goodness_of_fit_ref   1.695
_refine_ls_hydrogen_treatment    mixed
_refine_ls_matrix_type           full
_refine_ls_number_parameters     28
_refine_ls_number_reflns         841
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      1.695
_refine_ls_R_factor_all          0.0888
_refine_ls_R_factor_gt           0.0873
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[σ²(Fo²)+(0.1000P)²+0.0000P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.2543
_refine_ls_wR_factor_ref         0.2573
_reflns_number_gt                821
_reflns_number_total             841
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            sn0021-16.7d3.cif
_cod_data_source_block           16.7d3
_cod_depositor_comments
;
 Correcting the reference to the optimal entry by changing it from
 '2103518' to '2103517'. The reference now correctly refers to the
 entry with the lowest _refine_ls_R_factor_all value.

 Antanas Vaitkus,
 2018-11-16

The _diffrn_ambient_pressure was taken from the original data block
header, after comparison with the paper text and supplementary
material.

When more than one structure was present in the sn0021.cif file for a
given pressure, the structure with the minimal _refine_ls_R_factor_all
value was taken as the best one, and all others marked with the
'_cod_suboptimal_structure yes' tag.

Changing (with the help of Perl) all _diffrn_radiation_source values in
the files that were reportedly colected on the HASYLAB D3 beamline
(Hamburg) from 'fine-focus sealed tube' to synchrotron.

The command was:

perl -i -ne \
    "s/'fine-focus sealed tube'/synchrotron/; \
    print unless /_diffrn_radiation_type|_diffrn_radiation_monochromator/" \
    *d3*.cif \
    11.57split.cif \
    21.85split.cif \
    22.85split.cif

Saulius Gra\<zulis

 Removed the _cod_suboptimal_structure data item in preparation for
 its deprecation. The fact that the structure is a suboptimal one
 should be derived from the presence of the _cod_related_optimal_struct
 data item.

 Antanas Vaitkus,
 2019-05-21
;
_cod_related_optimal_struct      2103517
_cod_database_code               2103518
loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
'y, x, -z'
'-y, x-y, z'
'-x+y, -x, z'
'-x, -x+y, -z'
'x-y, -y, -z'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_symmetry_multiplicity
_atom_site_calc_flag
_atom_site_refinement_flags
La La 0.4382(3) 0.0000 0.0000 0.0292(4) Uani 1 2 d S
Ga1 Ga 0.0000 0.0000 0.0000 0.0313(6) Uani 0.50 6 d SP
Ta Ta 0.0000 0.0000 0.0000 0.0313(6) Uani 0.50 6 d SP
Ga2 Ga 0.6667 0.3333 -0.5121(9) 0.0276(8) Uani 1 3 d S
Ga3 Ga 0.0000 -0.2340(4) -0.5000 0.0252(5) Uani 1 2 d S
O1 O 0.6667 0.3333 -0.168(5) 0.023(3) Uiso 1 3 d S
O2 O 0.154(5) -0.294(6) -0.309(8) 0.093(12) Uiso 1 1 d .
O3 O 0.227(3) 0.079(4) -0.232(4) 0.056(5) Uiso 1 1 d .
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
La La -0.9400 1.6200 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Ta Ta -0.9400 4.4000 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Ga Ga 0.2490 1.0600 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0028 0.0036 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
O3 La O3 65.9(11) 6 .
O3 La O1 77.7(6) 6 2_545
O3 La O1 122.9(6) . 2_545
O3 La O1 122.9(6) 6 .
O3 La O1 77.7(6) . .
O1 La O1 157.30(12) 2_545 .
O3 La O2 138.1(9) 6 4_655
O3 La O2 107.9(12) . 4_655
O1 La O2 72.1(8) 2_545 4_655
O1 La O2 93.5(7) . 4_655
O3 La O2 107.9(12) 6 2_655
O3 La O2 138.1(9) . 2_655
O1 La O2 93.5(7) 2_545 2_655
O1 La O2 72.1(8) . 2_655
O2 La O2 102.4(17) 4_655 2_655
O3 La O2 63.9(10) 6 6
O3 La O2 77.4(11) . 6
O1 La O2 123.8(10) 2_545 6
O1 La O2 66.3(9) . 6
O2 La O2 158.0(7) 4_655 6
O2 La O2 64.2(15) 2_655 6
O3 La O2 77.4(11) 6 .
O3 La O2 63.9(10) . .
O1 La O2 66.3(9) 2_545 .
O1 La O2 123.8(10) . .
O2 La O2 64.2(15) 4_655 .
O2 La O2 158.0(7) 2_655 .
O2 La O2 133.8(13) 6 .
O3 La Ga2 108.9(6) 6 2_544
O3 La Ga2 85.3(6) . 2_544
O1 La Ga2 66.3(6) 2_545 2_544
O1 La Ga2 110.2(5) . 2_544
O2 La Ga2 31.5(8) 4_655 2_544
O2 La Ga2 132.2(8) 2_655 2_544
O2 La Ga2 162.6(8) 6 2_544
O2 La Ga2 32.7(7) . 2_544
O3 La Ga2 85.3(6) 6 1_556
O3 La Ga2 108.9(6) . 1_556
O1 La Ga2 110.2(5) 2_545 1_556
O1 La Ga2 66.3(6) . 1_556
O2 La Ga2 132.2(8) 4_655 1_556
O2 La Ga2 31.5(8) 2_655 1_556
O2 La Ga2 32.7(7) 6 1_556
O2 La Ga2 162.6(8) . 1_556
Ga2 La Ga2 163.40(7) 2_544 1_556
O3 La Ga1 33.0(5) 6 .
O3 La Ga1 33.0(5) . .
O1 La Ga1 101.35(6) 2_545 .
O1 La Ga1 101.35(6) . .
O2 La Ga1 128.8(9) 4_655 .
O2 La Ga1 128.8(9) 2_655 .
O2 La Ga1 66.9(7) 6 .
O2 La Ga1 66.9(7) . .
Ga2 La Ga1 98.30(3) 2_544 .
Ga2 La Ga1 98.30(3) 1_556 .
O3 La Ta 33.0(5) 6 .
O3 La Ta 33.0(5) . .
O1 La Ta 101.35(6) 2_545 .
O1 La Ta 101.35(6) . .
O2 La Ta 128.8(9) 4_655 .
O2 La Ta 128.8(9) 2_655 .
O2 La Ta 66.9(7) 6 .
O2 La Ta 66.9(7) . .
Ga2 La Ta 98.30(3) 2_544 .
Ga2 La Ta 98.30(3) 1_556 .
Ga1 La Ta 0.0 . .
O3 Ga1 O3 88.3(9) 4 .
O3 Ga1 O3 81.8(14) 4 5
O3 Ga1 O3 164.0(15) . 5
O3 Ga1 O3 103.9(14) 4 6
O3 Ga1 O3 81.8(14) . 6
O3 Ga1 O3 88.3(9) 5 6
O3 Ga1 O3 164.0(15) 4 2
O3 Ga1 O3 103.9(14) . 2
O3 Ga1 O3 88.3(9) 5 2
O3 Ga1 O3 88.3(9) 6 2
O3 Ga1 O3 88.3(9) 4 3
O3 Ga1 O3 88.3(9) . 3
O3 Ga1 O3 103.9(14) 5 3
O3 Ga1 O3 164.0(15) 6 3
O3 Ga1 O3 81.8(14) 2 3
O3 Ga1 La 128.0(7) 4 2
O3 Ga1 La 98.0(7) . 2
O3 Ga1 La 98.0(7) 5 2
O3 Ga1 La 128.0(7) 6 2
O3 Ga1 La 40.9(7) 2 2
O3 Ga1 La 40.9(7) 3 2
O3 Ga1 La 40.9(7) 4 4
O3 Ga1 La 128.0(7) . 4
O3 Ga1 La 40.9(7) 5 4
O3 Ga1 La 98.0(7) 6 4
O3 Ga1 La 128.0(7) 2 4
O3 Ga1 La 98.0(7) 3 4
La Ga1 La 120.0 2 4
O3 Ga1 La 98.0(7) 4 .
O3 Ga1 La 40.9(7) . .
O3 Ga1 La 128.0(7) 5 .
O3 Ga1 La 40.9(7) 6 .
O3 Ga1 La 98.0(7) 2 .
O3 Ga1 La 128.0(7) 3 .
La Ga1 La 120.0 2 .
La Ga1 La 120.0 4 .
O3 Ta O3 88.3(9) 4 .
O3 Ta O3 81.8(14) 4 5
O3 Ta O3 164.0(15) . 5
O3 Ta O3 103.9(14) 4 6
O3 Ta O3 81.8(14) . 6
O3 Ta O3 88.3(9) 5 6
O3 Ta O3 164.0(15) 4 2
O3 Ta O3 103.9(14) . 2
O3 Ta O3 88.3(9) 5 2
O3 Ta O3 88.3(9) 6 2
O3 Ta O3 88.3(9) 4 3
O3 Ta O3 88.3(9) . 3
O3 Ta O3 103.9(14) 5 3
O3 Ta O3 164.0(15) 6 3
O3 Ta O3 81.8(14) 2 3
O3 Ta Ga3 157.9(7) 4 3_556
O3 Ta Ga3 96.5(7) . 3_556
O3 Ta Ga3 88.3(7) 5 3_556
O3 Ta Ga3 55.9(7) 6 3_556
O3 Ta Ga3 32.4(7) 2 3_556
O3 Ta Ga3 113.3(7) 3 3_556
O3 Ta Ga3 113.3(7) 4 2
O3 Ta Ga3 157.9(7) . 2
O3 Ta Ga3 32.4(7) 5 2
O3 Ta Ga3 88.3(7) 6 2
O3 Ta Ga3 55.9(7) 2 2
O3 Ta Ga3 96.5(7) 3 2
Ga3 Ta Ga3 61.84(7) 3_556 2
O3 Ta Ga3 55.9(7) 4 2_554
O3 Ta Ga3 88.3(7) . 2_554
O3 Ta Ga3 96.5(7) 5 2_554
O3 Ta Ga3 157.9(7) 6 2_554
O3 Ta Ga3 113.3(7) 2 2_554
O3 Ta Ga3 32.4(7) 3 2_554
Ga3 Ta Ga3 145.49(4) 3_556 2_554
Ga3 Ta Ga3 107.22(9) 2 2_554
O3 Ta Ga3 88.3(7) 4 3
O3 Ta Ga3 32.4(7) . 3
O3 Ta Ga3 157.9(7) 5 3
O3 Ta Ga3 113.3(7) 6 3
O3 Ta Ga3 96.5(7) 2 3
O3 Ta Ga3 55.9(7) 3 3
Ga3 Ta Ga3 107.22(9) 3_556 3
Ga3 Ta Ga3 145.49(4) 2 3
Ga3 Ta Ga3 61.84(7) 2_554 3
O3 Ta Ga3 32.4(7) 4 .
O3 Ta Ga3 55.9(7) . .
O3 Ta Ga3 113.3(7) 5 .
O3 Ta Ga3 96.5(7) 6 .
O3 Ta Ga3 157.9(7) 2 .
O3 Ta Ga3 88.3(7) 3 .
Ga3 Ta Ga3 145.49(4) 3_556 .
Ga3 Ta Ga3 145.49(4) 2 .
Ga3 Ta Ga3 61.84(7) 2_554 .
Ga3 Ta Ga3 61.84(7) 3 .
O3 Ta Ga3 96.5(7) 4 1_556
O3 Ta Ga3 113.3(7) . 1_556
O3 Ta Ga3 55.9(7) 5 1_556
O3 Ta Ga3 32.4(7) 6 1_556
O3 Ta Ga3 88.3(7) 2 1_556
O3 Ta Ga3 157.9(7) 3 1_556
Ga3 Ta Ga3 61.84(7) 3_556 1_556
Ga3 Ta Ga3 61.84(7) 2 1_556
Ga3 Ta Ga3 145.49(4) 2_554 1_556
Ga3 Ta Ga3 145.49(4) 3 1_556
Ga3 Ta Ga3 107.22(9) . 1_556
O1 Ga2 O2 119.4(12) . 2_654
O1 Ga2 O2 119.4(12) . 6_554
O2 Ga2 O2 97.9(16) 2_654 6_554
O1 Ga2 O2 119.4(12) . 5_664
O2 Ga2 O2 97.9(16) 2_654 5_664
O2 Ga2 O2 97.9(16) 6_554 5_664
O1 Ga2 La 136.39(6) . 4_664
O2 Ga2 La 103.8(13) 2_654 4_664
O2 Ga2 La 43.3(14) 6_554 4_664
O2 Ga2 La 54.6(11) 5_664 4_664
O1 Ga2 La 136.38(6) . 2_654
O2 Ga2 La 54.6(11) 2_654 2_654
O2 Ga2 La 103.8(13) 6_554 2_654
O2 Ga2 La 43.3(14) 5_664 2_654
La Ga2 La 73.37(9) 4_664 2_654
O1 Ga2 La 136.38(6) . 1_554
O2 Ga2 La 43.3(14) 2_654 1_554
O2 Ga2 La 54.6(11) 6_554 1_554
O2 Ga2 La 103.8(13) 5_664 1_554
La Ga2 La 73.37(9) 4_664 1_554
La Ga2 La 73.37(9) 2_654 1_554
O1 Ga2 La 42.23(5) . 4_665
O2 Ga2 La 160.6(12) 2_654 4_665
O2 Ga2 La 90.1(11) 6_554 4_665
O2 Ga2 La 98.4(14) 5_664 4_665
La Ga2 La 94.152(11) 4_664 4_665
La Ga2 La 140.165(6) 2_654 4_665
La Ga2 La 140.164(6) 1_554 4_665
O1 Ga2 La 42.23(5) . .
O2 Ga2 La 90.1(11) 2_654 .
O2 Ga2 La 98.4(13) 6_554 .
O2 Ga2 La 160.6(12) 5_664 .
La Ga2 La 140.164(6) 4_664 .
La Ga2 La 140.163(6) 2_654 .
La Ga2 La 94.152(11) 1_554 .
La Ga2 La 71.20(8) 4_665 .
O1 Ga2 La 42.23(5) . 2_655
O2 Ga2 La 98.4(13) 2_654 2_655
O2 Ga2 La 160.6(12) 6_554 2_655
O2 Ga2 La 90.1(11) 5_664 2_655
La Ga2 La 140.165(6) 4_664 2_655
La Ga2 La 94.152(11) 2_654 2_655
La Ga2 La 140.163(6) 1_554 2_655
La Ga2 La 71.20(8) 4_665 2_655
La Ga2 La 71.20(8) . 2_655
O2 Ga3 O2 106(3) 5_554 .
O2 Ga3 O3 98.4(17) 5_554 6_554
O2 Ga3 O3 106.5(17) . 6_554
O2 Ga3 O3 106.5(17) 5_554 4
O2 Ga3 O3 98.4(17) . 4
O3 Ga3 O3 138.3(15) 6_554 4
O2 Ga3 Ta 85.8(13) 5_554 1_554
O2 Ga3 Ta 142.2(14) . 1_554
O3 Ga3 Ta 35.8(7) 6_554 1_554
O3 Ga3 Ta 112.9(8) 4 1_554
O2 Ga3 Ta 142.2(14) 5_554 .
O2 Ga3 Ta 85.8(13) . .
O3 Ga3 Ta 112.9(8) 6_554 .
O3 Ga3 Ta 35.8(7) 4 .
Ta Ga3 Ta 107.22(9) 1_554 .
O2 Ga3 La 86.5(13) 5_554 2_545
O2 Ga3 La 36.1(14) . 2_545
O3 Ga3 La 140.8(7) 6_554 2_545
O3 Ga3 La 74.7(7) 4 2_545
Ta Ga3 La 170.48(8) 1_554 2_545
Ta Ga3 La 82.30(2) . 2_545
O2 Ga3 La 36.1(14) 5_554 2_544
O2 Ga3 La 86.5(13) . 2_544
O3 Ga3 La 74.7(7) 6_554 2_544
O3 Ga3 La 140.8(7) 4 2_544
Ta Ga3 La 82.30(3) 1_554 2_544
Ta Ga3 La 170.48(8) . 2_544
La Ga3 La 88.18(8) 2_545 2_544
Ga2 O1 La 109.9(6) . 4_665
Ga2 O1 La 109.9(6) . .
La O1 La 109.0(6) 4_665 .
Ga2 O1 La 109.9(6) . 2_655
La O1 La 109.0(6) 4_665 2_655
La O1 La 109.0(6) . 2_655
Ga3 O2 Ga2 118(2) . 2_544
Ga3 O2 La 117.8(17) . 2_545
Ga2 O2 La 105.2(17) 2_544 2_545
Ga3 O2 La 116.9(18) . .
Ga2 O2 La 92.6(12) 2_544 .
La O2 La 102.7(14) 2_545 .
Ga3 O3 Ta 111.8(12) 3 .
Ga3 O3 Ga1 111.8(12) 3 .
Ta O3 Ga1 0.0 . .
Ga3 O3 La 139.7(12) 3 .
Ta O3 La 106.1(10) . .
Ga1 O3 La 106.1(10) . .
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
La O3 2.35(2) 6
La O3 2.35(2) .
La O1 2.472(9) 2_545
La O1 2.472(9) .
La O2 2.40(4) 4_655
La O2 2.40(4) 2_655
La O2 2.75(4) 6
La O2 2.75(4) .
La Ga2 3.369(3) 2_544
La Ga2 3.369(3) 1_556
La Ga1 3.450(2) .
La Ta 3.450(2) .
Ga1 O3 1.95(2) 4
Ga1 O3 1.95(2) .
Ga1 O3 1.95(2) 5
Ga1 O3 1.95(2) 6
Ga1 O3 1.95(2) 2
Ga1 O3 1.95(2) 3
Ga1 La 3.450(2) 2
Ga1 La 3.450(2) 4
Ta O3 1.95(2) 4
Ta O3 1.95(2) .
Ta O3 1.95(2) 5
Ta O3 1.95(2) 6
Ta O3 1.95(2) 2
Ta O3 1.95(2) 3
Ta Ga3 3.1050(18) 3_556
Ta Ga3 3.1050(18) 2
Ta Ga3 3.1050(18) 2_554
Ta Ga3 3.1050(18) 3
Ta Ga3 3.1051(18) .
Ta Ga3 3.1051(18) 1_556
Ga2 O1 1.72(3) .
Ga2 O2 1.82(3) 2_654
Ga2 O2 1.82(3) 6_554
Ga2 O2 1.82(3) 5_664
Ga2 La 3.369(3) 4_664
Ga2 La 3.369(3) 2_654
Ga2 La 3.369(3) 1_554
Ga2 La 3.457(3) 4_665
Ga2 La 3.457(3) 2_655
Ga3 O2 1.78(3) 5_554
Ga3 O2 1.78(3) .
Ga3 O3 1.79(2) 6_554
Ga3 O3 1.79(2) 4
Ga3 Ta 3.1050(18) 1_554
Ga3 La 3.592(3) 2_545
Ga3 La 3.592(3) 2_544
O1 La 2.472(9) 4_665
O1 La 2.472(9) 2_655
O2 Ga2 1.82(3) 2_544
O2 La 2.40(4) 2_545
O3 Ga3 1.79(2) 3
